View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
Properties of MBE-Grown ZnBeSe: Studyof Be Isoelectronic Traps and of Dopant BehaviorI.L. Kuskovsky1Þ (a), Y. Gu (a), M. van der Voort (a), C. Tian (a), B. Kim (a),I.P. Herman (a), G.F. Neumark (a), S.P. Guo (b), O. Maksimov (b),and M.C. Tamargo (b)(a) Department of Applied Physics and Applied Mathematics, Columbia University,New York, NY 10027, USA(b) Chemistry Department, City College of CUNY, New York, NY 10007, USA(Received July 27, 2001; accepted September 30, 2001)Subject classification: 71.35.–y; 71.55.Gs; 78.55.Et; 78.66.Hf; S8.12In this paper we present studies on undoped, Cl-doped, and N-doped ZnBeSe using photolumines-cence (PL). We show that the dominant PL from undoped samples is ‘‘effective mass” type andsuggest that it is of isoelectronic origin. We also show that the binding energy of both donor andacceptor impurities increases with Be concentration.Introduction II–VI wide bandgap semiconductors are of high interest for fabricatingdevices emitting light in the green and blue spectral regions. However, such deviceshave short ‘‘lifetimes” . The use of Be in ZnSe based alloys (i.e. Zn1ÀxBexSe ternaryalloy) has been suggested  to improve the hardness of the material [3, 4], and as aresult the device lifetime. In this paper we present PL studies of both undoped anddoped ZnBeSe that shed some light on the nature of the luminescent transitions ofthese materials.Undoped ZnBeSe Our samples are nominally undoped, grown by molecular beamepitaxy (MBE). For the details of the growth procedure see Guo et al. . The domi-nant feature in all samples consists of a strong, fairly sharp line (sometimes consistingof two peaks, with a splitting less than 3 meV) in the near band edge region withseveral weaker lines on the low-energy side, and, at least in samples with less than 6%Be, two lines on the high-energy side . (Samples with Be concentrations higher than6% do not show these two peaks due to larger lattice mismatch.) We attributed thedominant line to bound excitons, the peaks on the low energy side to phonon replicasof the main peak(s), and the high energy peaks to free excitons , with their locationgiving the excitonic bandgap.To further understand the possible origin of the dominant PL features, we performedPL temperature (T) and pressure (P) studies. We plot in Figs. 1a and b the peak en-ergy as a function of temperature and pressure, respectively. The temperature depen-dence was fitted to Varshni’s formula, EðTÞ ¼ Eð0Þ À aPLT2=ðbPL þ TÞ (see Ref. ),giving aPL ¼ 9:0 Â 10À4eV/K and bPL ¼ 365K, which are very close to values obtainedearlier for the ZnSe [8, 9] bandgap. The pressure dependence was fitted to a quadraticformula, EðPÞ ¼ Eð1 atmÞ þ aPP þ bPP2, where aP and bP are the linear and quadraticphys. stat. sol. (b) 229, No. 1, 239–243 (2002)# WILEY-VCH Verlag Berlin GmbH, 13086 Berlin, 2002 0370-1972/02/22901-0239 $ 17.50þ.50/01) Corresponding author; Tel.: 1-212-854-1580; Fax: 1-212-854-8257; e-mail: email@example.com
pressure coefficients, respectively. This resulted in aP ¼ 6:61 meV/kbar andbP ¼ À1:1 Â 10À2meV/(kbar)2, i.e. values which are very close to those obtained forthe pressure shift of the ZnSe bandgap [10, 11]. These two observations mean that thedefect responsible for the PL is of ‘‘effective mass” nature, since it is well known thatin the ‘‘effective mass” approximation all relevant states are formed from the bandwavefunctions and, thus, all energy levels follow the band edge with temperature andpressure.Thus, both temperature and pressure studies show ‘‘effective mass” behavior, eventhough the exciton has a larger ionization energy. According to Ref.  ZnBeSe is acompletely miscible system and we do not believe that the same atom can both changethe bandgap and also create a localized level. Thus, we suggest that a complex of Beintroduces an isoelectronic trap, and therefore the observed PL is due to isoelectronicbound excitons. Since the Be atom is substantially smaller than Zn, it is quite probablethat Be will introduce a short-range potential which would lead to the formation of anisoelectronic trap . Moreover, since the ionization energy of Be is slightly smallerthan that of Zn, according to the theory of Hopfield et al.  this would lead tohaving the trap capturing a hole first, with an electron subsequently captured via theCoulomb attraction, i.e. there is formation of an isoelectronic donor. Such a donor isexpected to be effective mass like , and the observed effective mass behavior in ourexperiments confirms that this is indeed the case.Doped ZnBeSe Figure 2 shows PL data from three typical ZnBeSe:Cl samples. It isplausible to assume that the observed PL is due to neutral donor (Cl) bound excitons.It is interesting to compare the peak positions of the bound excitonic line with reportedZnBeSe bandgap values. There are several reports on the dependence of the ZnBeSedirect bandgap, e.g.  or the excitonic bandgap, e.g. [6, 12, 16] on Be concentration.(We would like to note that the data in Ref.  are referred to as the bandgap; how-ever, the ZnSe data-point of 2.80 eV clearly suggests that the obtained dependenceprovides the excitonic bandgap.) In Refs. [12, 16] similar dependences of the bandgapon composition of 23 and 24 meV per %, respectively, were reported. In Ref.  thebandgap values were obtained at room temperature via absorption experiments andhave only four data-points. The best fit of these data can be obtained if a quadratic240 I.L. Kuskovsky et al.: Properties of MBE-Grown ZnBeSe: Isoelectronic TrapsFig. 1. Peak position of the domi-nant PL from undoped ZnBeSeas a function of a) temperature;b) pressure
dependence on the Be composition is assumed. Similarly, a quadratic dependence wasreported in Ref. .Since Refs. [15, 16] pertain to bulk crystals, for our comparison we shall use onlydata from Refs. [6, 12] corrected for the binding energy of the ZnSe free exciton(20 meV).The peak position for the sample with 1% Be is about 2:827 eV, while the corre-sponding bandgap values are 2:845 eV with use of  and 2:857 eV with . Thus, thePL peak is below the edge of the bandgap by 18 meV if we use Ref.  and by30 meV if we use Ref. . Clearly, 18 meV is an unrealistic number since it is smallerthan the free exciton binding energy (20 meV in ZnSe); on the other hand, 30 meVseems quite realistic (the position of the Cl bound exciton is 25–26 meV below theZnSe band edge); moreover, one expects an increase of the excitonic binding energy inZnBeSe due to a decrease of the dielectric function. Indeed, the binding energy of ahydrogenic impurity would increase as the dielectric constant decreases with the in-crease of the bandgap due to the higher Be concentration. (A simple theory, see e.g., predicts that dielectric constant decreases as a square of the bandgap.) When weconsider the 3:3% Be sample, the peak here is at 2:877 eV while the bandgaps valuesreported are 2:898 eV  and 2:916 eV . Again, the separation calculated using thefirst value is 21 meV, which appears too small, while the second value gives 40 meV,which we believe is more likely. (Both approaches give a larger binding energy for the2:7% Be sample, which admittedly we find puzzling.)We, however, note that the range of our data is for samples with relatively low Beconcentrations, since at higher Be content the binding energy of free excitons is ex-pected to increase, and the observed bending  of the excitonic bandgap would notrepresent a real bandgap value. Thus we suggest that an extension of this investigationtoward higher Be content material is needed.Next we show in Fig. 3a low temperature PL from a typical uniformly dopedZn0:966Be0:034Se:N sample at different excitation intensities (normalized and shiftedalong intensity axis for convenience). The high excitation intensity spectrum consists ofa dominant peak at 2:769 eV and a shoulder at 2:746 eV as well as a small high energypeak at 2:844 eV. It is clear that the peak at 2:746 eV is not a phonon replica of thephys. stat. sol. (b) 229, No. 1 (2002) 241Fig. 2. Low temperature PL fromthree ZnBeSe:Cl samples; the in-set show the peak position as afunction of Be concentration forall investigated samples
dominant transition as it does not scale with the intensity of the 2:769 eV peak; more-over, it becomes dominant at lower excitation intensities. In Fig. 3b we show the energydifference between the dominant peak energy and the bandgap calculated according toRefs.  and . In both cases the binding energies of the relevant impurities increasewith Be content. This corresponds to hydrogenic nature of the impurities as has alreadybeen mentioned above. Note that in the similar case of ZnMgSe:N such a behaviorwas not observed, but rather several discrete values for N acceptor were reported, de-pending on the number of surrounding Mg atoms .If we extrapolate these data to ZnSe values we obtain the following values: 81 meVif we use Ref.  and 105 meV if we use Ref. . We note that previously this PL wasattributed to a donor–acceptor pair (DAP) recombination [6, 18]. Therefore, we canestimate a sum of the activation energies of acceptors and donors, EA þ EDð Þ, by add-ing to the above values the Coulomb shift. We take a Coulomb shift of about 25 meV,which is appropriate for a shallow donor in ZnSe . With this Coulomb shift weobtain EA þ EDð Þ % 106 meV, using Ref.  and EA þ EDð Þ % 130 meV, using Ref. . Itis clear that the latter values are closer to those expected for ZnSe ( EA þ EDð Þ % 137 meVfor a 111 meV acceptor and a 26 meV donor).Therefore, giving the results for Cl and N doped samples, the bandgap values re-ported in Ref.  seem too low to explain the observed PL, at least in the case of lowBe concentrations. We, therefore, postulate that the bandgap of ZnBeSe first increasessuperlinearly, but then it may well become a linear function of Be concentration, asreported elsewhere .Summary We have investigated the behavior of undoped and doped ZnBeSe alloysystem with Be concentrations less than 6%. We have found that the dominant radia-tive transition in undoped material is of isoelectronic nature. Also, from a donor boundexcitonic PL as well as a lower energy DAP band, we conclude that the impurity activa-tion energies increase with Be concentration according to the ‘‘effective mass” approx-imation. Our data also suggest that the behavior of ZnBeSe bandgap as a function ofBe composition requires further investigation.242 I.L. Kuskovsky et al.: Properties of MBE-Grown ZnBeSe: Isoelectronic TrapsFig. 3. a) Intensity dependence ofthe PL from a typical ZnBeSe:Nsample; b) energy separation ofthe dominant peak from the band-gap calculated using Ref.  (cir-cles) and Ref.  (triangles)
Acknowledgement We would like to acknowledge support from NSF (grant # DMR-98-05760) for this work.References S. Itoh, K. Nakano, and A. Ishibashi, J. Cryst. Growth 214/215, 1029 (2000). A. Waag, Th. Litz, F. Fischer, H.-J. Lugauer, T. Baron, K. Schull, U. Zehnder, T. Gerhard,U. Lunz, M. Keim, G. Reuscher, and G. Landwehr, J. Cryst. Growth 184/185, 1 (1998). C. Verie, J. Cryst. Growth 184/185, 1061 (1998). K. Maruyama, K. Suto, and J.-I. Nishizawa, J. Cryst. Growth 214/215, 104 (2000). S. P. Guo, Y. Luo, W. Lin, O. Maksimov, M. C. Tamargo, I. Kuskovsky, C. Tian, and G. F.Neumark, J. Cryst. Growth 208, 205 (2000). I. Kuskovsky, C. Tian, G.F. Neumark, S.P. Guo, and M.C. Tamargo, J. Cryst. Growth 214/215,1058 (2000). Y.P. Varshni, Physica 34, 149 (1967). Y. Shirakawa and H. Kukimoto, J. Appl. Phys. 51, 2014 (1980). K.A. Bowers, Z. Yu, K.J. Gossett, J.W. Cook, Jr., and J.F. Schetzina, J. Electron. Mater. 23,251 (1994). J.A. Tuchman, S. Kim, Z. Sui, and I.P. Herman, Phys. Rev. B 46, 13371 (1992). M. Ming Li, D. J. Strachan, T. Ritter, M. Tamargo, and B. A. Weinstein, Phys. Rev. B 50,4385 (1994). C. Chauvet, E. Tournie´, and J.P. Faurie, J. Cryst. Growth 214/215, 95 (2000). W. Allen, J. Phys. C 4, 1936 (1971). J.J. Hopfield, D.G. Thomas, and R.T. Lynch, Phys. Rev. Lett. 17, 312 (1966). J. Zakrzewski, F. Firszt, S. Łegowski, H. Meczyn´ska, B. Sekulska, J. Szatkowski, and W. Pasz-kowicz, Microelectron. J. 31, 821 (2000). A. Bakaluk, A.A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Łegowski, H. Mec-zyn´ska, and J. Szatkowski, Appl. Surf. Sci. 175/176, 531 (2001). J.M. Ziman, Principles of the Theory of Solids, Cambrifdge University Press, Cambridge 1965. E. Tournie and J.-P. Fourie, Appl. Phys. Lett. 75, 382 (1999). C. Morhain, D. Seghier, B. Vo¨gele, C. O’Donnell, K.A. Prior, B.C. Cavenett, and H.P. Gislason,J. Cryst. Growth 214/215, 482 (2000). G.F. Neumark, L. Radomsky, and I. Kuskovskiy, Proc. SPIE 2346, 159 (1994).phys. stat. sol. (b) 229, No. 1 (2002) 243